Selective separation and purification of cerium (III) from concentrate liquor associated with monazite processing by cationic exchange resin as adsorbent

The present study is directed to find the optimal conditions required for efficient separation and purification of Ce3+ as an analog for lanthanides from Fe3+, Th4+, and Zr4+ (interfering ions) using Amberlite IR120H (AIR120H) resin as a strongly cationic exchange adsorbent. The main factors affecting the separation processes had been investigated and optimized. Ce3+ (Ln3+) as an admixture with Fe3+, Th4+, and Zr4+ was successfully separated by batch and column techniques. The sorption efficiency (S, %) from different acidic media was in this order: HCl > HNO3 > H2SO4. In a quaternary mixture with Fe3+ and Th4+, the maximum separation factor between Ce3+ and Zr4+ was ~ 13 after 90 min of equilibration, and the sorption capacity of AIR120H resin for Ce3+ was 8.2 mg/g. The rate of adsorption was found to follow a pseudo-second-order kinetic model. Separation of the absorbed ions was achieved by desorption processes. Firstly, 98 ± 2% of loaded Ce3+ is fully desorbed by 1 M sodium acetate solution without interfering ions. Moreover, ~ 95% of Zr4+ is desorbed by 1 M citric acid solution. Finally, 85% of loaded Fe3+ and Th4+ ions are desorbed with 8 M HCl solution. The batch technique was applied to separate and purify Ln3+-concentrate in chloride liquor (LnCl3), coming from the caustic digestion of Egyptian high-grade monazite. However, the enhanced radioactivity in LnCl3 due to radium -isotopes (228Ra2+, 226Ra2+, 224Ra2+, 223Ra2+) and radio-lead (210Pb2+) is initially reduced by a factor of 92% (i.e., safe limit) by pH-adjustment. As result, it can be recommended that the sorption process by AIR120H resin is efficient and promising for exploring pure lanthanides from its minerals.


Introduction
The degree of purity of lanthanides (Ln 3+ , 4f-elements) plays a significant role in many areas of contemporary techniques. Lanthanides have many scientific applications such as catalysts, synthetic products and a variety of applications in nuclear energy (Du and Graedel 2011;Tian et al. 2012;Metwally and Rizk 2014). Therefore, the production of lanthanides with high purity is very important for such applications. Variable minerals are considered the main sources of lanthanides such as monazite (light Ln-PO 4 ) (Borai et al. 2017a, b) bastnaesite (Ln-FCO 3 ) and xenotime (heavy Ln-PO 4 ) (Rosenblum and Fleischer 1995). Separation of lanthanides from these minerals is usually after concentration, leaching and filtration. The problem is the selective as well as quantitative separation of lanthanides in the presence of impurities from the post-filtration solution. The separation of lanthanides from the most abundant rare earth mineral, i.e., monazite ore is usually associated with impurities such as U(IV), Th(IV), Fe(III), and Zr(IV) (Hamed et al. 2016). The effective separation and purification of lanthanides from these impurities is thus an interesting step. Most of the studies under this aim usually utilize the traditional precipitation method (Abreu and Morais 2010;Borai et al. 2018;Kumari et al. 2018;Rodliyah et al. 2015). The disadvantages of the precipitation method are that more time is spent in digest, filtering, or washing and disposal the precipitates, limited recovery of rare earths, highly dependent on pH that Ln 3+ can co-precipitate with Th and U with any error in the detection of the pH value, and pollution from the storage of radioactive precipitate (Ang et al. 2018;Wang et al. 2013). On the other hand, the ion exchange technique is the most suitable separation technique due to its non-complication as associated with solvent extraction due to less use of organic solvent and less waste accumulation (Mayyas et al. 2014;Rizk et al. 2022a;Rodríguez et al. 2016;Shu et al. 2018;Zhang et al. 2004) and overcomes the traditional precipitation method problems, as well as the ability of ion exchangers and chelating resins to extract Ln 3+ from dilute solution (Esma et al. 2014). Monazite is the main source of lanthanides and thorium in the world. In Egypt, monazite contains on average 50% lanthanide as Ln 2 O 3 . The concentration of cerium in Ln 2 O 3 cake was ~ 45% (Ali et al. 1996). So, recovery and separation of lanthanides from monazite-cake require quantitative removal of the interfering metal ions as Zr 4+ , Th 4+ or Fe 3+ . Therefore, the efficiency of Amberlite IR120H resin as a cation exchanger for separation and purification of Ce 3+ as analog for lanthanides from Zr 4+ , Th 4+ , and Fe 3+ , commonly exist in monazite, with high purity and yield were studied to determine the optimum conditions for separation of Ce 3+ from these undesirable ions using batch and column technique. Further, the obtained optimum conditions will be applied to separate and purify Ln(III)-concentrate from the caustic digestion of Egyptian high-grade monazite.

Materials and reagents
All reagents used were of high analytical grade and used without further purification. Herein, the solid phase extraction is done by strongly cationic exchanger resin, Amberlite IR120H resin as AIR120H. The chemical structure of the AIR120H resin is represented in Fig. 1

Sorption experiments
Experiments of the solid phase extraction by AIR120H resin have been done to evaluate the feasibility of separation of Ce 3+ as analog for lanthanides (Ln 3+ ) from the undesired metal ions, e.g., Fe 3+ , Th 4+ and, Zr 4+ . The sorption experiments were performed assuming 100 ppm for each metal ion in all the studied solution systems (single or quaternary). In batch investigations, 5 mL of the prepared metal ion solution is mixed with 0.05 g of AIR120H resin, i.e., V/m is 0.1 L/g at room temperature. The parameters of sorption efficiency (S, %), sorption capacity (mg/g), distribution coefficient (K d , mL/g) and separation factor (SF) were defined by the next empirical formulas (El Afifi et al. 2016;Dakroury et al. 2020): where C o and C e are the initial and final concentrations of metal ions, respectively, while V and m represent the solution volume (L) and adsorbent mass (g). Moreover, the extraction chromatography had also been carried out using a glass column with 8 mm (internal diameter, ) and 100 mm (length l) with constant flow rate of 0.5 mL/min. Also, several solutions were examined for the desorption process of the loaded metal ions onto the resin. All experiments were Fig. 1 The chemical structure of AIR120H resin (Attallah et al. 2020)

Instrumentation
The initial and final concentrations of the studied metal ions were measured by a Cintra UV-visible spectrophotometer; model Cintra 2.2 (model Cintra 2.2, Australia). However, concentrations of Ce 3+ and Zr 4+ were measured as colored complexes by Arsenazo-III method at wave lengths of λ max 650 ± 2 and 665 ± 2 nm, respectively (Marczenko 1976). The concentration of Th 4+ was measured by the Thoron-I method as colored complex at 540 ± 2 nm, while Fe 3+ was measured by thiocyanate method at 495 ± 2 nm (Marczenko 1976). On the other hand, the radiometric measurements were done using multichannel NaI(Tl) scintillation detector and high purity germanium detector, Canberra Industries Inc. (USA) (Wang et al. 2015). The metal concentrations of LnCl 3 after deactivation were measured using ICPS-7500 (Shimadzu Sequential Plasma Spectrometer, Japan). The possible speciation diagrams of the metal ions have been done in HCl solution using HYDRA-MEDUSA-32 software (version 2009, Sweden) (Dakroury et al. 2020). The hydrogen ion concentration of the working solutions was adjusted using 0.1 M HCl or NaOH by pH-meter with accuracy of ± 0.1.

Results and discussion
Exploration of monazite mineral to obtain lanthanides as a strategic product face two opportunities, these are how to minimize the major undesired metallic impurities (e.g., Fe, Zr, Th) associated with lanthanides (Ln 3+ ) in the chloride liquor and the enhanced natural radioactivity due to presence radium-isotopes ( 228 Ra, 226 Ra, 223 Ra) and radio-lead ( 210 Pb 2+ ). Therefore, the required conditions for the efficient separation of lanthanides were investigated assuming simulated solutions containing Ce 3+ as analog for lanthanides and Fe 3+ , Th 4+ and Zr 4+ as interfering metal ions commonly exist in monazite or its corresponded Ln(III)-liquors. Hence, the optimized conditions will be applied for the purification of real lanthanide liquor from the enhanced natural radioactivity level and the undesired metallic impurities.

Factors affecting the separation conditions
Some factors had been investigated to find sorption behavior of Ce 3+ ions and the interfering metal ions, e.g., Fe 3+ , Th 4+ and Zr 4+ by AIR120H resin as strongly cationic adsorbent. Thus, different parameters included acid solution type, acid concentration, and equilibration periods were studied to find the optimum conditions required for the efficient separation of Ce 3+ from the interfering metal ions (Fe 3+ , Th 4+ , Zr 4+ ) of our interest, as listed below.

Acid solution type
For this purpose, the sorption behavior of 5 ml from100 ppm Ce 3+ (i.e., Ln 3+ ) as well as Fe, Th and Zr was investigated individually in different acidic solutions of 0.1 M HCl, HNO 3 and H 2 SO 4 solutions, using 0.05 g of AIR120H resin with contact time, 2 h and room temperature. The results are given in Fig. 2. It is observed that the sorption efficiency (S, %) of the metal ions was significantly varied with the investigated acid solution type in accordance as HCl > HNO 3 > H 2 SO 4 . The lower sorption efficiency from H 2 SO 4 media may be related to the dissociation of sulfuric acid giving two hydrogen atoms that compete with the cation on the active site of the resin. On the other hand, the removal efficiency from hydrochloric acid is more favorable than nitric acid may be due to the higher electronegativity of NO 3 − than for Cl − ion and may be masking for the cations. The increase in the sorption efficiency of Amberlite IR120 resin from HCl more than HNO 3 has been mentioned also in our previous work (Rizk et al. 2022b).

Concentration of HCl solutions
The influence of HCl solutions on the sorption behavior of all the studied metal ions (100 ppm) and contact time, 2 h, is investigated within the concentration range 0.001-5 M. The sorption process is done individually by the used AIR120H resin. The results are illustrated in Fig. 3.
It is observed that the S, % of all metal ions is high in diluted solutions (0.001-0.1 M HCl), then, decreased gradually to1 M, followed by a rapid decrease to 5 M HCl. The sorption behavior of Ce, Fe and Th is almost similar compared to Zr. The S, % of Ce, Fe and, Th was in the average 95 ± 2% within 0.001-0.1 M HCl, while it was about 40 ± 3% for Zr. Over 0.1 M HCl leads to a significant decrease in the S, %. It is found that the S, % of Ce, Fe, Th and Zr at 1 M HCl solution is decreased to 72 ± 3, 65 ± 2, 58 ± 2 and 18 ± 2%, respectively. On the other hand, the S, % of all metal ions was nil at 5 M HCl, Fig. 3. The decrease in the S, % may be due to a larger competition between the positively charged species of the studied metals with protons as result of the high acid concentration to be chelated with resin sulfonic moieties (El Afifi et al. 2016; Rizk and El-Hefny 2020). Thus, 0.01 M HCl (pH 2) is chosen as suitable and efficient solution for sorption of the metal ions in the next investigations. As reported by Hamed et al., this value of pH (pH 2) was suitable for selective separation of Fe 3+ from U 4+ , Th 4+ , and Ce 3+ using nanocomposite of polyaniline functionalized Tafa (Hamed et al. 2019). To know the sorption mechanism between the studied metal ions with active sites of the used AIR120H resin, speciation diagrams of Ce 3+ , Fe 3+ , Th 4+ , and Zr 4+ have been constructed in Fig. 4a-d. It is observed that all metal ions were adsorbed onto the resin as a result of the ion exchange process between the resin sulfonic moieties, i.e., -SO 3 H, and the positively charged species of the metal ions. Regarding Fig. 3, the high S, % was obtained at 0.001-0.1 M HCl (i.e., pH 1-3); this means that the metal ions created a positively charged species with the resin sulfonic moieties, i.e., -SO 3 H. Thus, Ce ions are adsorbed by ion exchange interaction as Ce 3+ , CeCl 2+ and/or CeCl 2 + ( Fig. 4a) with the resin moieties. This concept can be also said for the other metal ions, i.e., Fe 3+ or Th 4+ , with AIR120H resin moieties with pH's < 3, however, Fe 3+ ions exist as species of Fe 3+ , FeOH 2+ , FeCl 2+ and/ or FeCl 2 + (Fig. 4b); Th ions present as different species as Th 4+ , ThCl 3+ , ThOH 3+ , ThCl 2 2+ or Th(OH) 2 2+ (Fig. 4c); Zr exists as species of Zr 4 (OH) 8 8+ , Zr 3 (OH) 5 7+ , Zr 4+ , ZrOH 3+ , Zr(OH) 2 2+ or Zr(OH) 3 + (Fig. 4d). As seen in Fig. 4d, presence of bigger and bulkier positively charged species of Zr like Zr 4 (OH) 8 8+ and/or Zr 3 (OH) 5 7+ , as well as the higher free energy of hydration for Zr, may explain the lower affinity of Amberlite IR-120 toward Zr (Rizk et al. 2022b). It is common knowledge that metals have a stronger tendency to stay in the liquid phase and hydrate more water molecules as their absolute hydration free energy increases (Xu et al. 2021;Wang et al. 2020;Speight 2005). The free energy of hydration for Zr is higher than that for Th, Fe, and Ce (Wang et al. 2020;Mokhtari and Keshtkar 2016;Talebi et al. 2017). Therefore, Zr is more likely than Th, Fe, and Ce to remain in the liquid phase more than adsorbed in the resin. The possible ion exchange mechanism for sorption of the metal ions with AIR120H resin can be simply represented as

Equilibration periods
It is well known that contact time is one of the predominant factors governing the distribution of the metal ions between two phases. (Satusinprasert et al. 2015). The sorption behavior of Ce 3+ , i.e., Ln 3+ , is investigated with Fe 3+ , Th 4+ and Zr 4+ as interfering metal ions in admixture to simulate the presence of lanthanides in monazite matrix or its corresponded lanthanide chloride liquor (LnCl 3 ). The sorption performance of the investigated ions in admixture from 0.01 M HCl solution was conducted at different intervals ranging from 15 to 120 min. and V/m ratio of 0.1 L/g at 25 ± 1 °C. Figure 5 shows that the S, % of all metal ions from admixture is decreased than from single  Table 2. It is observed that the all sorption parameters (S, %-sorption capacity, mg/g-K d , mL/g-SFs) of the studied metal ions are increased through the first 30 min., followed by a slow increase till one hour. Therefore, 90 min. is enough time to attain constant equilibration for the studied metal ions. Hence, the maximum S, % at 90 min was ~ 82 ± 2% for Ce 3+ ~ Fe 3+ ~ Th 4+ and was about 26 ± 2% for Zr 4+ . The initial fast increase in the sorption parameters may be due to the existence of numerous vacant active sites on the surface of AIR120H resin at the initial stage, which was occupied by the metal ions with the increase in the contact time .
The values of the SFs between Ce 3+ (i.e., Ln 3+ ) and Zr 4+ are rapidly increased till one hour, then, the high SF values are attained within equilibration periods of 1-2 h. Thus, the maximum SF between Ce 3+ and Zr 4+ in quaternary admixture with Fe 3+ and Th 4+ was 12.98 at an equilibration period of 90 min, Table 2. Further, the results at equilibrium are compared with those reported elsewhere in the literature. Regarding the sorption capacity obtained herein, it is found that the sorption capacity of Ce 3+ found by AIR120H resin (q e , 8.2 mg/g) was larger than that reported by Jian et al., (q e , 2.5 mg/g) (Jain et al. 2001), close to that found by Gok et al. (2007) (q e , 8.3 mg/g) and below that reported by Bhatt et al. (2014) (q e , 86.4 mg/g) for sorption of Ce 3+ using different sorbents. The variations between the obtained results herein and those reported can be due to differences in their experimental conditions. In the case of separation factor, the values of separation factor of Ce 3+ are still very limited by solid phase extraction (SPE). Herein, the SF value of Ce 3+ /Zr 4+ is low relative to those reported by Eusebius et al. (1977) to separate Ce 3+ from Ce 4+ and UO 2   Table 3. As can be seen from the previous results, separation of Ce 3+ was not achieved yet. Therefore, the desorption process for separation of Ce 3+ from majority Fe 3+ , Th 4+ , and minors of Zr 4+ loaded onto AIR120H resin is investigated below.

Adsorption kinetic study
After studying appropriate contact time for adsorption of Ce 3+ , Fe 3+ , Th 4+ , and Zr 4+ using AIR120H resin, it is important to establish the sorption kinetic models in order to examine the controlling mechanism of the adsorption process. Therefore, the experimental sorption data were analyzed using the linear form of pseudo-first-order (Lagergren 1898) Eq. (7), pseudosecond-order (Ho and Mckay 1999) Eq. (8).
In these formula, q e and q t are the concentration of the metal ion sorbed at equilibrium and at time t (mg/g) and k 1 (min −1 ) and k 2 (g/mg min) are the pseudo-first-order and second-order rate constant, respectively. The initial sorption rate, h (mg/g min) at t → 0, is calculated using the secondorder rate constant k 2 as follows: Figure 6a, b shows the results of the two kinetic models, and their kinetic parameters are given in Table 4. It was demonstrated that good linear correlation factor (R 2 ) values were obtained for both the first and second kinetic models, especially for adsorption of Fe 3+ and Th 4+ , but that pseudosecond-order achieved closer agreement between theoretical and experimental q e values for all investigated ions. These findings demonstrate that the pseudo-second-order kinetics for the whole sorption period accurately describes the sorption data. These data imply that the chemisorption process appears to be in control of the overall rate of these metal ions adsorption process (Patawat et al. 2020;Pathania et al. 2017). The exterior liquid film diffusion, surface adsorption, and intra-particle diffusion processes that coexisted during adsorption are also explained by this model (Fan et al. 2017;Patawat et al. 2020).

Desorption investigation
The desorption process is mainly aimed at liberating Ce 3+ , i.e., Ln 3+ , separately without interfered metal ions (Fe 3+ , Th 4+ and Zr 4+ ) as possible. For this purpose, several solutions including double distilled water (DDW) and 1 M of  . 6 The pseudo-first-order (a) and second-order kinetic (b) for adsorption of Ce 3+ , Fe 3+ , Th 4+ and Zr 4+ ions on AIR120H resin. 25 ± 0.3 °C sodium chloride, citric acid, sodium sulfate, sodium acetate, hydrochloric acid, and ammonium thiocyanate solutions had been examined for desorption of the metal ions loaded onto the AIR120H resin. Firstly; quaternary admixtures of Ce, Fe, Th and Zr (100 ppm for each) were prepared in 0.01 M HCl solution, then, loaded onto the AIR120H resin for equilibration after 90 min assuming V/m ratio of 0.1 L/g at room temperature. However, the resin-loaded by metal ions is filtered off and submitted for desorption process. Secondly; the loaded resin samples were desorbed by equilibrated with 5 mL of the examined solution for 90 min (V/m) ratio of 0.1 L/g at room temperature. Then, the desorption efficiency (D, %) of certain metal ion from the AIR120H resin is calculated according to (Rizk and El-Hefny 2020): where C L and C D represent concentration of the adsorbed and desorbed metal ions, respectively. The values of D, % using several solutions as eluents are given in Table 5. It is found that desorption of the loaded metal ions was nil by using double distilled water (DDW), HCl, or NH 4 SCN solutions. Further, 47 ± 1% and 98 ± 2% of adsorbed Ce 3+ are desorbed by using 1 M of NaCl and Na 2 SO 4 solutions but contaminated with 90% and 95% of Zr 4+ as an interfered metal ion using both solutions, respectively. Next, 98 ± 2%, i.e., 80.4 ± 1.6 ppm of Ce 3+ is fully desorbed by  observed that the D, % increases sharply with an increase in the concentration of the eluent till reaches equilibrium. As a results, 1 M of sodium acetate solution is suitable and efficient for desorption of Ce 3+ ions as a pure solution without interfering with metal ions of Fe 3+ , Th 4+ or Zr 4+ .

Column technique
Assuming the subsequent conditions for sorption and desorption of Ce 3+ in quaternary admixture with Fe 3+ , Th 4+ and Zr 4+ by batch technique, the solid phase extraction (SPE) is examined by column technique using AIR120H resin as cationic exchange as adsorbent. For this purpose, a pre-cleaned glass column ( ∅= 8 mm, L = 100 mm) is packed with a pre-conditioned AIR120H resin by double distilled water (DDW) for 24 h. The height of the resin in the column was adjusted to 4 ± 0.1 cm, and a steady flow rate of 0.5 mL/min of DDW, then 0.01 M HCl solution (2 × 15 mL) was used to condition the column. The column is kept wet before use. An admixture containing Ce 3+ (i.e., Ln 3+ ) with Fe 3+ , Th 4+ and Zr 4+ (100 ppm for each) is prepared in 0.01 M HCl solution. An accurate 5 mL of the admixture solution is loaded onto the pre-conditioned column resin bed (AIR120H). For desorption process, the column bed is rinsed by 3 × 5 mL of sodium acetate solution (1 M) then citric acid (1 M) and followed by 8 M HCl solution (used for the flushing process of the column resin after the elution process), with a constant flow rate of 0.5 mL/min. Hence, the effluents associated with the loading and elution processes of the column resin were measured to evaluate the amount of metals loaded onto the column resin or eluted from the column itself. The obtained results for loading and elution through the suggested column resin technique are demonstrated in Fig. 9. It is found that the loading efficiency (L, %) of the metal ions onto the column resin was 69 ± 4, 65 ± 3, 67 ± 4 and 21 ± 2% for Ce 3+ , Fe 3+ , Th 4+ and Zr 4+ , respectively. On the other hand, the desorption data indicated that Ce 3+ 95 ± 5% (i.e., 65.6 ± 4 ppm) of loaded ions was only present in sodium acetate solution without contamination with Fe 3+ or Th 4+ or Zr 4+ . Next, 86 ± 6% (18.1 ± 1.3 ppm) of loaded Zr 4+ was eluted in citric acid solution, while the other metals, i.e., Fe 3+ and Th 4+ , were not present. Finally, 83% (i.e., ~ 54 and, 55.61 ppm) of loaded Fe and Th ions are eluted with 8 M HCl solution. Thus, Ce 3+ (Ln 3+ ) is successfully separated out the metal ions commonly interfered with lanthanides either by batch or column techniques. By comparison between the data obtained from bath and column techniques, it can be concluded that the S% and L% values, in addition to, the amount of metal ions yield, i.e., desorbed (D) or eluted (E) were varied. This result may be due to the variations in their experimental conditions, in which there are no agitation, stirring and/or equilibrium in column technique  Fig. 9 Column operations of loading and elution of Ce 3+ , Fe 3+ , Th 4+ and Zr 4+ admixture using IR120H resin (Rizk et al. 2022a). The amounts of metal ions separated by batch and column techniques are reported in Fig. 10.
(2) presence an enhanced natural radioactivity above the permitted limits (IAEA 2017); Table 7. Thus, the separation of Ln 3+ needs the next purification.

Removal of undesirable radionuclides
For this purpose, a sample of the high-grade monazite is digested by the caustic method. The produced hydroxide cake of Ln(III) is solubilized by hot concentrated HCl with stirring, then, it is filtered off to eliminate the non-reacted, suspended and/or insoluble matters. Hence, 1 mL of carrier solution containing 25 mg/mL of Ba 2+ and Pb 2+ is added to the lanthanide concentrate solution. Then, the lanthanides concentrate as LnCl 3 liquor is homogenized, adjusted to pH 2.5 ± 0.1, and left overnight. The mixture is filtered off to separate the 'insoluble residues' as a by-product away from the lanthanide concentrate as clear 'LnCl 3 liquor.' The radiometric measurements of the products indicated that ~ 92% of natural radioactivity due to Ra 2+ -isotopes

Separation of lanthanides from LnCl 3 liquor
One milliliter of the de-activated LnCl 3 liquor was evaporated till near dryness, then, the residue is dissolved again by 500 µL of concentrated HCl diluted by double distilled water till the pH of the solution reached pH 2 ± 0.1 (i.e., 0.01 M HCl). Assuming the previously optimized conditions assuming batch investigations, 10 mL of the diluted LnCl 3 mixed with 0.1 g of AIR120H resin (V/m 0.1 L/g and at room temperature) was shaken for 90 min. The mixture is filtered off. Further, the loaded AIR120H resin is equilibrated again with 1 M sodium acetate solution to desorb the loaded Ln 3+ . Next, the solution was filtered off; the previous step was repeated with the same sample of the resin using 8 M hydrochloric acid solution for flushing the used AIR120H resin. Lanthanides and Th were selectively measured before and after equilibration of LnCl 3 liquor with the used resin and the solutions used for the subsequent desorption process. The concentration of the total Ln 3+ and Th 4+ in the prepared real sample was 92 and 14.2 ppm, respectively. After equilibration with the resin, the sorption % of total Ln 3+ and Th 4+ were about 82 ± 2% (~ 75.4 ppm Ln 3+ ) and 1 3 81 ± 2%, (~ 11.5 ppm Th 4+ ), respectively. After the desorption investigations, only total Ln 3+ are detected in sodium acetate solution without Th 4+ . It is found that 90 ± 5% of total Ln 3+ , i.e., ~ 68 ppm Ln 3+ , was recovered in sodium acetate solution and 86 ± 4% of loaded Th ions was eluted after washing the AIR120H resin with 8 M HCl. Moreover, the ICP-OES measurement for sodium acetate confirmed the presence of Ce, La and Nd as major elements without interfering metal ions. Figure 11 shows the flowchart for separation and purification of lanthanides (Ln 3+ ) from monazite by Amberlite IR120H.

Conclusion
Briefly, the sorption and desorption processes in this study were verified under optimal conditions. The order of the sorption effectiveness (S, %) for several acidic media was HCl > HNO 3 > H 2 SO 4 . After 90 min of equilibration in a quaternary mixture containing Fe 3+ and Th 4+ , the maximum separation factor between Ce 3+ and Zr 4+ was ~ 13, and the sorption capacity of AIR120H resin for Ce 3+ was 8.2 mg/g. This work used pseudo-first-order and pseudo-second-order kinetic models to explain the adsorption mechanism. The findings demonstrate that these metal ions adhered to pseudo-second-order during their adsorption processes on AIR120H resin, indicating that liquid film diffusion, intra-particle diffusion, and surface adsorption coexisted. This study was successful in isolating Ce 3+ , an analog of lanthanides (Ln 3+ ), with 100% purity from undesirable ions such as Zr 4+ , Fe 3+ , and Th 4+ using AIR120H resin as a strongly cationic exchange whether from a simulated or actual sample of the highgrade monazite. Additionally, these undesirable ions were also successfully separated from one another by desorption using different eluents such as 1 M citric acid for desorption of loaded Zr 4+ and then the loaded Fe 3+ and Th 4+ ions were desorbed by 8 M HCl which also used for the flushing process of the column resin after the elution process. Therefore, after desorption of all the loaded ions and flushing the sample with 8 M HCl, the used sample of AIR120H resin can easily be reused. It is concluded that the AIR120H resin can be considered an efficient and promising cationic adsorbent to explore Ln 3+ -concentrate in the chloride liquor (LnCl 3 ) associated with monazite processing.
Funding Open access funding provided by The Science, Technology & Innovation Funding Authority (STDF) in cooperation with The Egyptian Knowledge Bank (EKB).

Conflict of interest
The authors declared that they have no conflict of interest.
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http:// creat iveco mmons. org/ licen ses/ by/4. 0/.